Evaluation of Antibacterial and Anticancer Characteristics of Silver Nanoparticles Synthesized from Plant Extracts of Wrightia tinctoria and Acacia chundra

The study showed the ability to synthesize environmentally friendly silver nanoparticles (AgNPs) using extracts from Wrightia tinctoria seeds and Acacia chundra stems. Surface plasmon resonance peaks in the UV-Vis absorption spectra of both plant extracts verified AgNP synthesis. The structural and morphological properties of the AgNPs were investigated using analytical techniques such as XRD, FTIR, TEM, and EDAX. The AgNPs have an FCC crystalline structure, according to XRD study, and their sizes range from 20 to 40 nm, according to TEM images. Based on the results, these plant extracts have been identified as suitable bioresources for AgNP production. The study also showed that both AgNPs had significant levels of antibacterial activity when tested on four different microbial strains using the agar-well diffusion method. The bacteria tested included two Gram-positive strains (Staphylococcus aureus and Micrococcus luteus) and two Gram-negative strains (Proteus vulgaris and Escherichia coli). Furthermore, the AgNPs were found to have a significant anticancer effect on MCF-7 cell lines, suggesting that they may be useful in therapeutic applications. Overall, this research highlights the potential of the plant extracts considered as a source for synthesizing eco-friendly AgNPs with potential applications in medicine and other fields.


Introduction
Nanotechnology enables the production of materials with a wide range of morphologies, dimensions, and chemical compositions, all of which fall within the range of 1-100 nanometers. Nanoparticles have a wide range of uses in electronics, biology, and medicine due to their optical, antibacterial, therapeutic, and catalytic capabilities [1,2]. Te higher the ratio of surface area to volume of the nanoparticles is, the more efcient they are in biological systems. Traditional methods of chemical and physical synthesis of nanomaterials require more time and involve the use of more hazardous reducing or stabilizing chemicals [1][2][3]. Plants contain bioactive components such as phenols, favonoids, saponins, glycosides, tannins, alkaloids, polysaccharides, proteins, terpenoids, amines, ketones, and aldehydes that act as reducing, stabilizing, and capping agents in the conversion of metal ions to metal nanoparticles. Hence, the use of plant resources will eliminate the need for toxic solvents and chemicals [1][2][3][4][5][6][7][8]. Te aforementioned issues can be addressed, and biocompatibility with nanoparticles can be obtained, by using plant extracts as reducers and stabilizers in the synthesis of ecologically friendly metallic nanoparticles [9,10].
Pharmaceuticals, coatings, biological labeling, and packaging are just few of the industries where nanoparticles might be useful [5][6][7][8][9]. Silver nanoparticles (AgNPs) have attracted a lot of attention from researchers. In spite of the fact that higher concentrations of silver are toxic, a number of studies [8][9][10] demonstrate that lower concentrations of AgNO 3 have superior chemical stability and catalytic activity, biocompatibility, and intrinsic therapeutic potential.
Researchers from every corner of the globe are interested in silver nanoparticles because of the remarkable antibacterial qualities that they possess. Tribal plants are revered in India as the ecosphere's equivalent of a botanical garden because they are used to treat a wide range of illnesses and physical distress and are also used as medicines. Te bulk of the country's rural population practices traditional Indian medicine, such as Ayurveda [11]. Te employment of nanoparticles in conjunction with well-known and extensively distributed traditional plants has thrown fresh light on the study of natural science. Tere have been a lot of studies conducted on how to make silver nanoparticles with potential anticancer and antibacterial action. Some examples include Arctium lappa fruit extract [3], Solanum melongena leaves [3], Taraxacum mongolicum leaves [3], red currants berries [4], alcoholic fower extracts [5], Pisum sativum L extracts [6], Mangifera indica seed extracts [7], berry extracts [9], Cucumis prophetarum leaf extracts [10], and Alpina katsumadai seed extract.
Te Wrightia tinctoria (Wt) tree is an Apocynaceae family member that is found in several places in India [12,13]. It is a deciduous tree of modest to medium size. Te seeds and the bark of this plant are both employed in the practice of traditional Indian medicine as a means of curing gastrointestinal conditions including diarrhea and dysentery. Tis plant's bark has been demonstrated to be useful in treating a range of diseases, including abdominal pain, skin infections, and wounds; it can even reverse the efects of snake venom [14]. Furthermore, the seeds of this plant have been shown to have aphrodisiac properties [12][13][14][15]. Wrightia tinctoria is mentioned in several traditional medicinal systems used in South Asia as a useful cure for the treatment of heart palpitations and excessive blood pressure. Previous studies on the Wrightia tinctoria plant discovered important chemical components such as alkaloids, triterpenoids, steroids, and favonoids [14]. Acacia catechu (Ac), commonly known as Katha or Karangali, is a wellknown medicinal shrub in India [14][15][16][17]. Catechins, favanol glycosides, favonal dimers, cafeine, and rhamnetin are some of the plant's helpful components [18]. Te antibacterial and wound-healing abilities of this plant have been studied. It is used alone or in combination with cinnamon or opium to treat chronic diarrhea. Acacia catechu water decoctions are commonly drunk as health beverages, particularly in the Indian state of Kerala and neighboring states in India's southern region [18,19]. Te water decoction is supposed to enhance skin complexion, cleanse the blood of pollutants, and boost the immune system. Te antiinfammatory qualities of stem bark extract are one of its pharmacological capabilities. When tested against the MCF-7 cell line, the methanolic extract of Acacia catechu stem bark was found to be efective as both an antioxidant and an anticancer agent [20]. Tis discovery was made possible because methanolic extraction is more stable than water extraction.
Our goal in this study is to develop an easy green synthesis of AgNPs using Wrightia tinctoria seeds and Acacia chundra stems. Te generated AgNPs were analyzed by UV-Vis spectroscopy, X-ray difraction (XRD), Fourier-transform infrared spectroscopy (FTIR), transmission electron microscopy (TEM), and energy dispersive X-ray spectroscopy (EDAX). All of the AgNPs' characteristics, including their crystalline nature, size, and surface features, were investigated. An investigation of the biological activities of biosynthesized AgNPs was conducted. We used the well difusion experiment to test the antibacterial activity of the AgNPs against both Grampositive (Micrococcus luteus and Staphylococcus aureus) and Gram-negative bacteria (Escherichia coli and Proteus vulgaris). Furthermore, the anticancer potential of the produced AgNPs has been investigated. Figure 1 presents the schematic representation of the experimental process.

Materials and Methods
All the reagents in this study were of analytical grade, used without further purifcation. Te Wrightia tinctoria (Wt) seeds were obtained in the SP. Kovil, Kancheepuram, and Acacia catechu (Ac) stem bark were collected from Chennai district. (Wt). Te seeds of the Wrightia tinctoria plant were thorough washings, frst with water from the running faucet, then with distilled water twice, to remove any dirt or other organic particles that may have contaminated them. Tey are left to air-dry in the shade for a period of 20 days before being ground into a powder using a standard blender. Te powder is kept in a container that is hermetically sealed and placed in the refrigerator. A 250 ml conical fask was flled with 10 g of powder and 200 ml of distilled water. Te solution was brought to a temperature of 60°C and then boiled for two hrs. After being allowed to cool, the extract solution was passed through a Whatman 41 flter to remove any particles that were still present. In the end, the Wt extract solution was retained for use after being stored in a refrigerator at a temperature of 40°C.

Preparation of Extract Using Stem of Acacia catechu (Ac).
Following a comprehensive cleaning, the stems of Acacia catechu were allowed to dry at room temperature. Te stem was cut into very small pieces, and then it was boiled for 20 min in a round-bottom fask containing 250 ml of distilled water. For the purpose of fltering the extract, Whatman No. 1 flter paper was utilized. Te produced extract was placed in storage for use in further studies.

Synthesis of AgNPs.
To convert the Ag + ions, 25 ml of the plant extract sample is combined with 100 ml of an aqueous solution that contains 1 nM of AgNO 3 [21]. After 24 hrs, the reaction mixture was settled to its fnal state. Silver nanoparticle production was inferred from the change in reaction mixture colour. To further separate the reaction mixture, it was centrifuged at 2,000 rpm for 10 min. After that, the AgNPs were separated from the sample by centrifuging it for and dispersed in acetone before being stored.

AgNP Characterization.
Te identifcation of silver nanoparticles was confrmed, and their physio-chemical properties were studied through several characterization methods. Te AgNP formation was confrmed by using a Shimadzu UV-1800 spectrophotometer. Te spectral data were collected in the 200-800 nm range. Te X-ray diffraction measurements were taken with a Bruker difractometer outftted with Cu radiation (�1.5406). For FTIR study, a Perkin Elmer spectrometer was used, and spectra were gathered in the 500-4000 cm −1 region. Te TEM study was performed using the JEOL JEM-2100 microscope. Te nanoparticle solution was dried on a copper matrix to prepare the samples for analysis.

Antibacterial Activity.
In this research, four bacterial strains were chosen: two Gram-positive (Micrococcus luteus and Staphylococcus aureus) and two Gram-negative (Proteus vulgaris and Escherichia coli) to assess the antibacterial effectiveness of the synthesized AgNPs using the Agar-well difusion method. Tese bacterium isolates were acquired from the National Chemical Laboratory in Pune, India, and were kept at 4°C until further use. Tese microorganisms are clinically important because they can induce a variety of diseases. Te AgNPs were synthesized in a 100% DMSO solution at four distinct concentrations (25,50,75, and 100 μg/ml). Each well received 100 μl of an enriched AgNP sample. To assess antibacterial efectiveness, the radius of the zone of inhibition around each well was determined. Tree diferent experiments were performed, and the average of the data was used to determine AgNPs' antibacterial efcacy.

Anticancer Activity.
Cancer is a hereditary illness that quickly disseminates throughout the body, causing irreparable damage to human tissue [18]. Breast cancer, which is the growth of malignant cells in the breast, is a signifcant cause of high female cancer mortality rates. In this work, the in vitro anticancer efects of SeWt-AgNPs and StAc-AgNPs were investigated on MCF-7 cell lines at varying dosages using the MTT test. Te National Centre for Cell Science in Pune, India, provided the MCF-7 breast cancer cell line that was used in this study. Cells were planted at a density of 1 × 10 4 /well in 96-well plates and allowed to grow for 24 hrs at 37°C in a humidifed atmosphere. After that, they were given an AgNP treatment at concentrations of 1.5, 6.25, 12.5, 50, and 100 μg/ml and placed in an incubator for 24 hrs. Te MTT test was used in accordance with the procedure to determine the level of viability shown by cells that had been treated with these compounds as well as those that had been left untreated (serving as a control). Te expression was what was used to determine whether or not the cells were viable. % viability � (mean absorbance of treated group) (mean absorbance of control group) × 100.
(1) Acacia catechu (Ac) International Journal of Analytical Chemistry (as shown in Figures 2(a) and 2(b)). Furthermore, no typical peaks were detected, suggesting that the solution did not contain an overabundance of starting materials. Tese fndings support earlier research by demonstrating the efective synthesis of AgNPs using plant extracts [21][22][23][24]. Rabaa Algotiml et al. [1] synthesized biogenic AgNPs from extracts of three distinct types of marine algae (green, brown, and red algae), and the absorption maxima were found to be at 424, 409, and 415 nm, respectively. Similarly, peaks at 420 nm were detected when the surface plasmon resonance (SPR) band of silver nanoparticles prepared using Calotropis procera latex was observed by a UV-Vis  International Journal of Analytical Chemistry spectrophotometer [23]. Previous research and the current results show the possibility of using plant extracts to make ecofriendly AgNPs with a variety of absorption spectra that can be used in a variety of uses, including medicine and technology.

XRD Studies.
Te X-ray difraction (XRD) is widely used to study the structural and crystalline properties of materials. Te structural properties of SeWt-AgNPs and StAc-AgNPs were investigated using XRD analysis in this study. Te XRD patterns found for both samples verifed the existence of a crystalline structure and matched the elemental silver face-centered cubic (FCC) lattice structure. Te appearance of four diferent peaks in the XRD spectra of SeWt-AgNPs (Figure 3(a)) at 27.78°, 32.19°, 46.2°, and 76.5°a nd StAc-AgNPs at 27.7°, 32.2°, 45.8°, and 76.5° (Figure 3(b)) showed the FCC crystal structure of the synthesized AgNPs. Some minor peaks in the XRD spectra were also detected, which could be ascribed to surface reactions of either biological or chemical origin. Te fndings of a number of other researchers were similar to the conclusion reached in the present investigation [3][4][5][6][7][8].

TEM Analysis.
Transmission electron microscopy (TEM) was utilized for the purpose of determining the morphology, shape, and size of nanoparticles. Figures 4(a) and 4(b) show the TEM micrograph of SeWt-AgNPs and StAc-AgNPs, respectively. It was discovered that the majority of the created AgNPs were in the shape of spheres. Te TEM pictures were processed with the image J program, which resulted in the creation of a histogram displaying the distribution of particle sizes. It has been determined that the diameters of SeWt-AgNPs and StAc-AgNPs are between 20 and 40 nm, with the former having a value that is considerably greater than the latter. SeWt-AgNPs had a median particle size of 39.75 nm ( Figure 5(a)) whereas the StAc-AgNPs had a median particle size of 27.79 nm ( Figure 5(b)).
In their study using seeds from the Mangifera indica plant, Donga and Chanda [7] found spherical AgNPs of varied sizes from 9 to 61 nm. Te extract of Alpinia katsumadai seed produced quasispherical AgNPs with an average particle size of 12 nm [12].

EDAX Spectra Analysis.
Energy dispersive X-ray spectroscopy, often known as EDAX, is a method that may be utilized to ascertain the elemental components that are present in the specimen. It was determined that surface Plasmon resonance was the cause of the absorption peak that was observed in the EDAX spectra (Figures 6(a) and 6(b)), which was located at around 2.5 keV. Tis provides more evidence that silver ions can be broken down into elemental silver [25].

Antibacterial Activity.
Against a diverse collection of microorganisms, the antibacterial efcacy of the AgNPs was evaluated at four distinct concentrations: 25, 50, 75, and 100 μg/ml (Figures 8 and 9). When compared to StAc-AgNPs, it has been demonstrated that SeWt-AgNPs possess antibacterial activity that is considerably less potent. At each concentration, the SeWt-AgNPs demonstrated their antibacterial activity. When Gram-negative bacteria were exposed to SeWt-AgNPs, they displayed an antibacterial

E. coli and Vibrio cholera
Reduction of microbial loading in drinking water [29] 5 International Journal of Analytical Chemistry activity that was remarkably similar to antibacterial activity of Gram-positive bacteria. When compared to their antibacterial activity against other bacteria, StAc-AgNPs have a level of efectiveness that is marginally higher against E. coli and B. subtilis. Te antibacterial activity varies based on the concentration of the nanoparticles as well as the type of bacteria being studied. All of the sensitive bacteria exhibit growth-restriction zones with a diameter that ranges from 11 mm to 20 mm. Silver nanoparticles are among the most signifcant metal nanoparticles because of their robust antibacterial capabilities. Because of these features, silver nanoparticles are among the most signifcant types of metal nanoparticles. Te AgNPs, which were produced from an aqueous extract of the outer peel of Pisum sativum, were shown to be bactericidal against four human pathogenic bacteria (with inhibition zones ranging from 8.70 to 11.10 mm on agar plates) [6]. It has been discovered that green silver nanoparticles (AgNPs) produced from an aqueous extract of Mangifera indica seeds are more efcient than traditional antibacterial treatments against Gramnegative bacteria [7]. Table 1 contains a discussion of the fndings of microbial efcacy of AgNPs produced from diferent plant extracts.

Anticancer Activity.
AgNP cell viability was measured using the MTT test. When delivered at concentrations between 1.5 and 100 μg/ml, both SeWt-AgNPs and StAc-AgNPs show signifcant cytotoxicity ( Figure 10). It was shown that both types of AgNPs were able to prevent the formation of cancer cells by the fact that the proliferation of the MCF cell line was dramatically decreased across the board. Light microscopy was used to examine the morphology of MCF-7 cancer cells after they had been incubated   with AgNPs for 24 hrs at doses of 1.5, 6.25, 12.5, 50, and 100 μg/ml (Figures 11 and 12). At concentrations of 1.5 μg/ ml of AgNPs, there are no discernible alterations in the morphology of the photos. However, at 6.25, 12.5, 50, and 100 μg/ml, AgNPs inhibited cell proliferation at a dosedependent rate. Tere was a noticeable shift in cell shape at both 50 and 100 μg/ml. Te results demonstrated a signifcant reduction in MCF-7 cell viability as compared to the plant extract. We can attribute this decline to the presence of AgNPs. Table 2 shows the fndings of a study contrasting the antineoplastic activity of the various natural sources used to produce AgNPs.

. Conclusions
Te Wrightia tinctoria seed extracts and the Acacia catechu stem extracts were both utilized during the course of this experiment to facilitate the synthesis of the AgNPs. UV-Vis spectrophotometry confrms the formation of AgNPs, and the XRD analysis reveals the FCC crystalline structure of the AgNPs. Te TEM micrographs demonstrated that the AgNPs had a spherical shape and that their diameters ranged from 20 to 40 nm. Te AgNPs were found to be uniformly distributed. Overall, the study has shown that plant extracts can be used as eco-friendly and cost-efective alternatives to traditional chemical methods for the synthesis of AgNPs. Te synthesized AgNPs showed promising antibacterial and anticancer activities, indicating their potential use in various biomedical applications. Further research is needed to explore the mechanisms of action and toxicity of these AgNPs and to optimize their synthesis parameters to enhance their properties for specifc applications.

Data Availability
Te data used in this study are included within the article.

Conflicts of Interest
Te authors declare that they have no conficts of interest.